DOI: 10.17188/1666507
title: Materials Data on Li7V3P8O29 by Materials Project

description: Li7V3P8O29 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are fourteen inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with three VO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 66–74°. There are a spread of Li–O bond distances ranging from 1.86–2.32 Å. In the second Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with three VO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 66–71°. There are a spread of Li–O bond distances ranging from 1.87–2.26 Å. In the third Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.14 Å. In the fourth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.99–2.12 Å. In the fifth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.94–2.15 Å. In the sixth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share a cornercorner with one LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.99–2.13 Å. In the seventh Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.95–2.18 Å. In the eighth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.92–2.11 Å. In the ninth Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with three VO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 67–68°. There are a spread of Li–O bond distances ranging from 1.86–2.24 Å. In the tenth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.93–2.20 Å. In the eleventh Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share a cornercorner with one LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.92–2.14 Å. In the twelfth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.23 Å. In the thirteenth Li1+ site, Li1+ is bonded in a 2-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.61 Å. In the fourteenth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.79 Å. There are six inequivalent V+3.67+ sites. In the first V+3.67+ site, V+3.67+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.87–2.00 Å. In the second V+3.67+ site, V+3.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with two LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 2.02–2.07 Å. In the third V+3.67+ site, V+3.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with two LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.84–2.02 Å. In the fourth V+3.67+ site, V+3.67+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra, corners with six PO4 tetrahedra, and edges with two LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.99–2.08 Å. In the fifth V+3.67+ site, V+3.67+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra and corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.86–2.03 Å. In the sixth V+3.67+ site, V+3.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with two LiO4 tetrahedra and corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.86–2.04 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 46–49°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 46–47°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with three LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 46°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 28–38°. There are a spread of P–O bond distances ranging from 1.50–1.58 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 24–36°. There are a spread of P–O bond distances ranging from 1.49–1.58 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 49°. There are a spread of P–O bond distances ranging from 1.52–1.60 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 40–47°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 47–49°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 41°. There are a spread of P–O bond distances ranging from 1.51–1.60 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with three LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 46–49°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–41°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and corners with three LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–39°. There are a spread of P–O bond distances ranging from 1.51–1.58 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 31–35°. There are a spread of P–O bond distances ranging from 1.49–1.59 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 44–45°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with three LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 44–46°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 41–45°. There are a spread of P–O bond distances ranging from 1.52–1.62 Å. There are fifty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a 2-coordinate geometry to two Li1+ and one P5+ atom. In the second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the third O2- site, O2- is bonded in a distorted trigonal planar geometry to two Li1+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+3.67+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the eighth O2- site, O2- is bonded in a trigonal planar geometry to two Li1+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+3.67+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the twelfth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+3.67+ and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a linear geometry to one Li1+ and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a linear geometry to one Li1+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+3.67+, and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.67+, and one P5+ atom. In the eighteenth O2- s